acts to stabilize the iron oxide and prevents sintering. The operation of HTS catalysts occurs within the temperature range of 310 °C to 450 °C. The temperature increases along the length of the reactor due to the exothermic nature of the reaction. As such, the inlet temperature is maintained at 350 °C to prevent the exit temperature from exceeding 550 °C. Industrial reactors operate at a range from atmospheric pressure to 8375 kPa (82.7 atm). The search for high performance HT WGS catalysts remains an intensive topic of research in fields of chemistry and materials science. Activation energy is a key criteria for the assessment of catalytic performance in WGS reactions. To date, some of the lowest activation energy values have been found for catalysts consisting of copper nanoparticles on ceria support materials, with values as low as Ea = 34 kJ/mol reported relative to hydrogen generation. Low temperature shift catalysis Catalysts for the lower temperature WGS reaction are commonly based on copper or copper oxide loaded ceramic phases, While the most common supports include alumina or alumina with zinc oxide, other supports may include rare earth oxides, spinels or perovskites. A typical composition of a commercial LTS catalyst has been reported as 32-33% CuO, 34-53% ZnO, 15-33% Al2O3. The active catalytic species is CuO. The function of ZnO is to provide structural support as well as prevent the poisoning of copper by sulfur. The Al2O3 prevents dispersion and pellet shrinkage. The LTS shift reactor operates at a range of 200–250 °C. The upper temperature limit is due to the susceptibility of copper to thermal sintering. These lower temperatures also reduce the occurrence of side reactions that are observed in the case of the HTS. Noble metals such as platinum, supported on ceria, have also been used for LTS. Mechanism The WGSR has been extensively studied for over a hundred years. The kinetically relevant mechanism depends on the catalyst composition and the temperature. Two mechanisms have been proposed: an associative Langmuir–Hinshelwood mechanism and a redox mechanism. The redox mechanism is generally regarded as kinetically relevant during the high-temperature WGSR (> 350 °C) over the industrial iron-chromia catalyst. Historically, there has been much more controversy surrounding the mechanism at low temperatures. Recent experimental studies confirm that the associative carboxyl mechanism is the predominant low temperature pathway on metal-oxide-supported transition metal catalysts. Associative mechanism In 1920 Armstrong and Hilditch first proposed the